Dental Research, Dental Clinics, Dental Prospects
Fissure sealant materials: Wear resistance of flowable composite resins Sohrab Asefi1* • Solmaz Eskandarion2 • Shadi Hamidiaval3 1
Orthodontist, Tehran, Iran Assistant Professor, Department of Dental Materials, School of Dentistry, Shahid Beheshti University of Medical Sciences, Tehran, Iran 3 Assistant Professor, Department of Oral and Maxillofacial Radiology, Faculty of Dentistry, Lorestan University of Medical Sciences, Khorramabad, Iran *Corresponding Author; E-mail: [email protected]
Received: 29 October 2015; Accepted: 4 July 2016 J Dent Res Dent Clin Dent Prospect 2016; 10(3):194-199 |doi: 10.15171/joddd.2016.031 This article is available from: http://dentistry.tbzmed.ac.ir/joddd © 2016 Asefi et al. This is an Open Access article published and distributed by Tabriz University of Medical Sciences under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
Abstract Background. Wear resistance of pit and fissure sealant materials can influence their retention. Wear characteristics of sealant materials may determine scheduling of check-up visits. The aim of this study was to compare wear resistance of two flowable composite resins with that of posterior composite resin materials.
Methods. Thirty-five disk-shaped specimens were prepared in 5 groups, including two flowable composite resins (Estelite Flow Quick and Estelite Flow Quick High Flow), Filtek P90 and Filtek P60 and Tetric N-Ceram. The disk-shaped samples were prepared in 25-mm diameter by packing them into a two-piece aluminum mold and then light-cured. All the specimens were polished for 1minute using 600-grit sand paper. The samples were stored in distilled water at room temperature for 1 week and then worn by two-body abrasion test using "pin-on-disk" method (with distilled water under a 15-Nload at 0.05 m/s, for a distance of 100 meter with Steatite ceramic balls antagonists). A Profilometer was used for evaluating the surface wear. Data were analyzed with the one-way ANOVA.
Results. Estelite Flow Quick exhibited 2708.9 ± 578.1 μm2 and Estelite Flow Quick High Flow exhibited 3206 ± 2445.1 μm2of wear but there were no significant differences between the groups. They demonstrated similar wear properties.
Conclusion. Estelite flowable composite resins have wear resistance similar to nano- and micro-filled and micro-hybrid composite resins. Therefore, they can be recommended as pit and fissure sealant materials in the posterior region with appropriate mechanical characteristics.
Key words: Dental restoration wear, composite resins, pit and fissure sealants.
he most common chronic disease during childhood is dental caries.1Occlusal cariescomprises80% of primary lesions of permanent teeth.2 Prevention of caries is important during developJODDD, Vol. 10, No. 3 Summer 2016
ment because caries may lead to speech, aesthetic and psychological problems, abnormal tongue habits and masticatory deficiencies.3 Monitoring of nutrition, regular oral hygiene, check-ups by a dentist and also use of fluoride products are preventive regimens for primary and perma-
Wear Resistance of New Flowable Composites 195
nent dental caries. Although fluoride can be effective in caries control for smooth surfaces, it is not very effective in preventing pit and fissures lesions. Therefore, pit and fissure sealant therapy is an effective method in preventing dental caries, especially during childhood and adolescent period. Although the occlusal surfaces of children’s teeth constitute almost 12.5% of total dental surfaces, 85% of total caries incidence is seen in these areas.4 Therefore, sealing of pits and fissures is an effective way for preventing occlusal dental caries. During the past decades, a lot of materials have been suggested for this purpose like glass- ionomers, resin-modified glass-ionomers and resin-based composites such as compomer or flowable composite resins. The critical characteristics of these materials are good fluidity and low viscosity. Also, fissure sealant materials should have good bond strength and sealing ability to remain intact during the servicing period. Some of the disadvantages of sealants are microleakage, fracture toughness and wear.5,6 Wear resistance is an important necessity for sealant materials because it can help determine scheduling of check-up visits for evaluating sealant integrity and intactness.7 Low wear resistance for sealants may lead to restoration loss or fracture and also increased roughness and more plaque accumulation, which may result in caries development.8 Composite resin filler characteristics can influence composite resin wear. As the filler content of composite resin increases, we can expect more wear resistance in it in comparison to unfilled resins like pit and fissure sealant materials.9 In recent years, many studies have revealed that flowable composite resins can have bond strength and sealing ability similar to fissure sealant materials10 while they can have better mechanical properties.11,12 Also it was shown that wear resistance of flowable composite resins improved compared with universal composite resins in recent years.13
To determine the wear resistance of Estelite flowable composite resin as a fissure sealant material in the posterior region, we conducted an experimental study to compare the wear of these flowable composite resins with that of universal and packable ones. These flowable composite resins were utilized with mono-dispersing supra-nano spherical fillers and RAP technology (Radical Amplified Photopolymerization) for better resin polymerization. This can be useful in determining sealant servicing time and in planning checkup appointments. Methods Ethics approval was not required because this was an in vitro study on dental materials. We conducted this in vitro study to compare wear resistance of two flowable composite resins: posterior universal and packable composite resins. A total of 35 specimens were prepared in 5 groups. The sample size was calculated based on the study of Yesil et al.14 Minitab software program was used by considering α = 0.05, β = 0.2, a standard deviation of 0.06 and 0.1 as the significance level. Therefore, 7 specimens were included in each group. The commercial composite resins used in this study are presented in Table 1. The Table shows the type, size and volume of composite resin fillers in each group. Two-body abrasion test was the selected way for wear assessment and in this procedure we chose pin-on-disk method.15Diskshaped specimens were prepared, measuring 25 mm in diameter; therefore, they were placed by a plastic carrier instrument or injected into customized twopiece aluminum molds with a gyrate space removed from the middle part. In order to pack and smooth the surface of composite resins, two thin glass blocks were used and the composite resins were curedfor 40 seconds from each side with a hand-held LED lightcuring unit (Ultralume LED 5, Ultradent, UT, USA) in an overlapping manner for initial curing. The laboratory light-curing device, GC Labolight LV III (GC America Inc., Alsip, IL, USA), was used for 60 seconds on each side of the specimens for making
Table 1. Composites groups used in the study Material (Manufacturer) ESTELITE Flow Quick (Tokuyama dental Corp.) ESTELITE Flow Quick High Flow (Tokuyama dental Corp.) Filtek P90 (3M ESPE) Filtek P60 (3M ESPE) Tetric N-Ceram (Ivoclar Vivadent)
Type of Filler
Bis-GMA, UDMA, TEGDMA
Silica- Zirconia Supra-nano mono-dispersing spherical
Silica- Zirconia Supra-nano mono-dispersing spherical
Siloxane, Oxirane Bis-GMA, UDMA, TEGDMA Bis-GMA, UDMA, TEGDMA
% Filler by Weight (Volume) 71(53)
Mean Particle size of Filler
Microfiller: 0.4 Nanofiller: 0.07 µm
Microfiller: 0.4 Nanofiller: 0.07 µm
Quartz Zirconium- silicate
0.5 µm 0.6 µm
St. Paul/ USA St. Paul/ USA
JODDD, Vol. 10, No. 3 Summer 2016
Asefi et al.
sure of the same conversion effect. Surface roughness was standardized by polishing specimens with 600-grit sandpapers for 1 minute. This size of sandpapers has been used in some related articles;14 therefore, 600-grit size was used manually in all the groups. Soluble ingredients were removed by storing the specimens in distilled water for one week at room temperature. The specimens were worn by pinon-disk device in Tribology Laboratory of Metallurgy School in Tehran University. This tribometer is calibrated according to ASTM G99 standard periodically. In the pin-on-disk device, an antagonist material was installed on the mandrel of the device and the prepared disk-shaped specimens were fixed on the other compartment of the device. The disks were rotated by an electrical motor in a circular pattern and the antagonist was loaded under a predetermined force which was controlled by a digital load cell automatically. Wear procedure was stopped after the predetermined distance. The composite resin specimens were worn against Steatite ceramic balls as antagonists (Hoechst Ceram Tec, Wunsiedel, Germany).16 They measured 5 mm in diameter. The specimens were worn under a 15-N force and at 0.05 m/s for a 100-meter distance. In order to evaluate the wear of specimens, a Profilometer (T8000, Hommelwerke, Germany) was use. The Profilometer measured surface roughness in the direction of a radius of the disk randomly and indirectly constructed a surface structure graph in micrometer scale. We could able calculate the area of wear groove in each section by scanning one of the disk’s radii randomly. We found the wear area of each specimen as a groove in its cross-section based on surface graph which was constructed by the Profilometer (Figure 1). By multiplying this wear area by circle perimeter of the wear track, the wear of each specimen was calculated. Data was analyzed with one-way ANOVA and PASW18 software (PASW 18, SPSS, Chicago, IL, USA). Statistical significance was set at P